 Добавил:
Upload Опубликованный материал нарушает ваши авторские права? Сообщите нам.
Вуз: Предмет: Файл:
Composite Materials for Aircraft Structures.pdf
Скачиваний:
441
Добавлен:
31.05.2015
Размер:
9.22 Mб
Скачать

# 6 Structural Analysis

## 6.1Overview

In this chapter, the basic theory needed for the determination of the stresses, strains, and deformations in fiber composite structures is outlined. Attention is concentrated on structures made in the form of laminates because that is the way composite materials are generally used.

From the viewpoint of structural mechanics, the novel features of composites (compared with conventional structural materials such as metals) are their marked anisotropy and, when used as laminates, their macroscopically heterogeneous nature.

There is a close analogy between the steps in developing laminate theory and the steps in fabricating a laminate. The building block both for theory and fabrication is the single ply, also referred to as the lamina. This is a thin layer of the material (typical thickness around 0.125 mm for unidirectional carbon/epoxy "tape" and 0.25 mm for a cross-ply fabric or "cloth") in which all of the fibers are aligned parallel to one another or in an orthogonal mesh. The starting point for the theory is the stress-strain law for the single ply referred to its axes of material symmetry, defined here as the 0 - 1 , 2, 3 material axes. In constructing a laminate, each ply is laid-up so that its fibers make some prescribed angle with a reference axis fixed in the laminate. Here the laminate axes will be defined as the x-, y-, and

z - a x e s .

All later calculations are made using axes fixed in the structure (the structural axes). In a finite element model, the material properties are usually entered in the material axes. The lay-up of the laminate is defined in the laminate axes. The laminate theory described in this chapter will indicate how the properties of the laminate are derived. The transformation from the laminate axes to the global structural axes is then completed during the solution process. Because the designer can select his own lay-up pattern (because the laminate stress-strain law will depend on that pattern), it follows that the designer can design the material (as well as the structure).

For more detailed discussions of the topics covered in this chapter, see Refs. 1-7. For background material on the theory of anisotropic elasticity, see Refs. 8 - 10 .

171

172COMPOSITE MATERIALS FOR AIRCRAFT STRUCTURES

## 6.2Laminate Theory

Classical laminate theory defines the response of a laminate with the following assumptions:

For two-dimensional plane stress analysis, the strain is constant through the thickness.

For bending, the strain varies linearly through the thickness.

The laminate is thin compared with its in-plane dimensions.

Each layer is quasi-homogeneous and orthotropic.

Displacements are small compared with the thickness.

The behavior remains linear.

With these assumptions satisfied, the laminate theory allows the response of a laminate to be calculated, engineering constants to be determined to substitute into standard formulas for stresses and deflections, and material properties of the laminate to be defined for substitution into finite element analysis as described in Chapter 16.

6.2.1Stress-Strain Law for a Single Ply in the Material Axes: Unidirectional Laminates

Consider a rectangular element of a single ply with the sides of the element parallel and perpendicular to the fiber direction (Fig. 6.1). Clearly, the direction of the fibers defines a preferred direction in the material; it is thus natural to introduce a cartesian set of material axes 0 - 1 , 2, 3 with the /-axis in the fiber direction, the 2-axis perpendicular to the fibers of the ply plane, and the 3-axis perpendicular to the plane of the ply. Here, interest is in the behavior of the ply when subjected to stresses acting in its plane, in other words, under plane stress conditions. These stresses (also referred to the material axes) will be denoted by trl, tr2, r12 and the associated strains by el,/32, and 712. (Note that in composite mechanics, it is standard practice to work with "engineering" rather than "tensor" shear strains.) Although a single ply is highly anisotropic, it is intuitively evident that the coordinate planes 012, 023, and 031 are those of material symmetry, there being a mirror image symmetry about these planes.

 I 02. ~2 r12,712 3

L ]~-~°I,~I

0 I

Fibres

Fig. 6.1 Material axes for a single ply.

 STRUCTURAL ANALYSIS 173

A material having three mutually orthogonal planes of symmetry is known as orthotropic. The stress-strain law for an orthotropic material under plane stress conditions, referred to the material axes, necessarily has the following form:

 1 -1)21 El 0 E2 t32 --1)12 1 o'2 (6.1) E1 0 'Y12 E2 T12 1 0 0

where: El, E2 = Young's moduli in the 1 and 2 directions, respectively; v12 = Poisson's ratio governing the contraction in the 2 direction for a tension in the 1 direction; rE1 = Poisson's ratio governing the contraction in the 1 direction for a tension in the 2 direction; G12 = (in-plane) shear modulus.

There are five material constants in equation (6.1), but only four of these are independent because of the following symmetry relation1:

 1)12 1)21 - - = - - ( 6 . 2 ) E1 E2

For unidirectional tape of the type being considered here, E 1is much larger than either E2 or G12because the former is a "fiber-dominated" property, while the latter are "matrix dominated". For a bi-directional cloth, E 1 = E2 and both are much larger than G12.For tape, 1)12is matrix dominated and is of the order of 0.3, whereas the contraction implied in 1)21is resisted by the fibers and so is much smaller.

The above equations are all related to a single ply but, because the ply thickness does not enter into the calculations, they also apply to a "unidirectional laminate" that is simply a laminate in which the fiber direction is the same in all of the plies. In fact, most of the material constants for a single ply are obtained from specimen tests on unidirectional laminates, a single ply being itself too thin to test conveniently.

For much of the following analysis, it is more convenient to deal with the inverse form of equation (6.1), namely

 I0-1 I IQll(0) Q12(0) 0 ~32 02 = Q12(0) Q22(0) 0 (6.3) ~'12 0 0 Q66(0) "Y12

where the Qij(O), commonly termed the reduced stiffness coefficients, are given by

 Qn(0) - E1 E2 Q22(0) - - 1 - 1 ) 1 2 1 ) 2 1 1 - - 1)121)21 1)21E1 (6.4) Q12(0) Q66(0) = G12 1)121)21 1 -

174 COMPOSITEMATERIALS FOR AIRCRAFT STRUCTURES

It is conventional in composite mechanics to use the above subscript notation for Q, the point of which becomes evident only when three-dimensional anisotropic problems are encountered. The subscript 6 is for the sixth component of stress or strain that includes three direct terms and three shear terms.

6.2.2Stress-Strain Law for Single Ply in Laminate Axes: Off-Axis Laminates

As already noted, when a ply is incorporated in a laminate, its fibers will make some prescribed angle 0 with a reference axis fixed in the laminate. Let this be the x-axis, and note that the angle 0 is measured from the x-axis to t h e / - a x i s and is positive in the counterclockwise direction; the y-axis is perpendicular to the x- axis and in the plane of the ply (See Fig. 6.2.). All subsequent calculations are made using the x - y , or "laminate" axes, therefore it is necessary to transform the stress-strain law from the material axes to the laminate axes. If the stresses in the laminate axes are denoted by trx, try, and "l~y,then these are related to the stresses referred to the material axes by the usual transformation equations,

 Dry I= ifS 2 C2 2csl[C S 0"2l1 (6.5) "lxy CS - - C S C2 - - S 2 "/'12

where c denotes cos 0 and s denotes sin 0. Also, the strains in the material axes are related to those in the laminate axes, namely, 8x, ey, and Yxy, by what is essentially the strain transformation:

 e 2 1 s 2 s csl[x1 (6.6) = c 2 - c s ey 3/12 - - 2 C S 2CS C2 - - S2 % y I Oy, ey ......_..=, rxy, 7xy / . / / / t / / / / Y l ~ / / . . . / / / / , / . / / A /~'~ / e / / / / / / / / " ~ / / / ~ aXo ~X / / / / / / / / / / / / / ~ / / / / i I f # /

Fibres

Fig . 6 . 2 L a m i n a t e a x e s f o r a s i n g l e ply .

 STRUCTURAL ANALYSIS 175

Now, in equation (6.5), substitute for oq, ~r2, and T12 their values as given by equation (6.3). Then, in the resultant equations, substitute for 81, 82, and Y12their values as given by equation (6.6). After some routine manipulations, it is found

that the stress-strain law in the laminate axes has the form

EoxxoooxsolEx1

 O'y = axy( O) Qyy( O) Qys( O) 8y (6.7) "rxy Qx~(O) Qy~(O) Qss(O) yxy where the Qij(O) are related to the Qij(O) by the following equations: iQxxollc4 2c2s2 s4 4c2s2j Qxy(O)| C2S2 C4 -'~ S4 C2S2 --4C2S 2 Qyy(O) ] = s 4 2c2s 2 c 4 4c2s 2 Qxs(O) ] c3s --¢S(C 2 -- S2) --CS 3 --2CS(C 2 -- S2) Qys(O) I cs3 cs(c2 - \$2) - c 3 s 2cs(c2 - s2) Qss(O) J c2s2 _ 2 c 2 s 2 c2s2 (c 2 - \$2)2

F Q ll (0) 7

 / Q~(o)/ (6.8) [_Q66(O) J

Observe that, in equation (6. 7), the direct stresses depend on the shear strains (as well as the direct strains), and the shear stress depends on the direct strains (as well as the shear strain). This complication arises because, for non-zero 0, the laminate axes are not axes of material symmetry and, with respect to these axes, the material is not orthotropic; it is evident that the absence of orthotropy leads to the presence of the Qx~and Qy~terms in equation (6. 7). Also, for future reference, note that the expressions for Qxx(O), Q,,y(O), Qyy(O)and Q~s(O)contain only even powers of sin 0 and therefore these quantities are unchanged when 0 is replaced by - 0. On the other hand, the expressions for Qx~ and Qy~ contain odd powers of sin 0 and therefore they change sign when 0 is replaced by - 0.

Analogous to the previous section, the above discussion has been related to a single ply, but it is equally valid for a laminate in which the fiber direction is the same in all plies. A unidirectional laminate in which the fiber direction makes a non-zero angle with the x-laminate-axis is known as an "off-axis" laminate and is sometimes used for test purposes. Formulas for the elastic moduli of an off-axis laminate can be obtained by a procedure analogous to that used in deriving equation (6. 7). Using equation (6.1) with the inverse forms of equations (6.5) and (6.6) leads to the inverse form of equation (6.7), in other words, with the strains expressed in terms of the stresses; from this result, the moduli can be written. Details can be found in most of the standard texts, for example page 54 of Ref. 3.

176 COMPOSITE MATERIALS FOR AIRCRAFT STRUCTURES

Only the result for the Y o u n g ' s modulus in the x direction, Ex,will be cited here:

 1(~_.~) c a + ( 1 2vle~c2s + (l~ s 4 ( 6 . 9 ) - - = 4 : el / \E2/ Ex

The variation o f Ex with 0 for the case of a c a r b o n / e p o x y off-axis laminate is shown in Figure 6.3. The material constants o f the single ply were taken to be

 E1 = 137.44GPa E2 = 11 . 71GPa Gl2 = 5 . 5 1 G P a 1)1 2 : 0.25 1)21 = 0.0213

It can be seen that the modulus initially decreases quite rapidly as the off-axis angle increases from 0°; this indicates the importance o f the precise alignment of fibers in a laminate.

6.2.3 Plane Stress Problems for Symmetric Laminates

One o f the most c o m m o n laminate forms for composites is a laminated sheet loaded in its own plane, in other words, under plane stress conditions. In order for out-of-plane bending to not occur, such a laminate is always made with a lay-up that is symmetric about the mid-thickness plane. Just to illustrate the type of symmetry meant, consider an eight-ply laminate comprising four plies that are to be oriented at 0 ° to the reference (x) axis, two plies at + 4 5 °, and two plies at - 45 °. An example o f a symmetric laminate would be one with the following ply sequence:

0 ° / 0 ° / + 4 5 ° / - 4 5 ° / - 4 5 o / + 4 5 o / 0 0 / 0 °

i

E X

(GPa)

50

 0 1 J J 0 ]0 6O 90

O f f ~ i s a~J!e (.rfi~-grlze~)

F i g . 6 . 3 E x t e n s i o n a l m o d u l u s o f f - a x i s l a m i n a t e .

 STRUCTURAL ANALYSIS 177

On the other hand, an example of an unsymmetric arrangement of the same plies would be:

O°lO°lO°lO°1+45°1-45°1+45ol-45 °

These two cases are shown in Figure 6.4 where z denotes the coordinate in the thickness direction.

6.2.3. I Laminat e Stiffnes s Matrix. Consider now a laminate comprising n plies and denote the angle between the fiber direction in the kth ply and the x laminate axis by Ok (with the convention defined in Fig. 6.2). Subject only to the symmetry requirement, the ply orientation is arbitrary. It is assumed that, when the plies are molded into the laminate, a rigid bond (of infinitesimal thickness) is formed between adjacent plies. As a consequence of this assumption, it follows that under plane stress conditions the strains are the same at all points on a line through the thickness (i.e., they are independent of z). Denoting these strains by ex, ey, and "Yxy,it then follows from equation (6. 7) that the stresses in the kth ply will be given by:

 O'x(k) = Q~ ( Ok)ex + axy( Ok)l?,y+ Qxs( Ok)3'xy ~ry(k) = Qxy( ODex + ayy( Ok)f,y + Qys( Ok)'Yxy (6.10) "rxy(k) = Qxs( Ok)ex + ays( Ok)Sy + Qss( Ok)Yxy The laminate thickness is denoted by t and the thickness of the kth ply is

hk -- hk-1 with hi defined in Figure 6.5. Assuming all plies are of the same thickness (which is the usual situation), then the thickness of an individual ply is simply t/n. Now consider an element of the laminate with sides of unit length parallel to the x- and y-axes. The forces on this element will be denoted by Nx, Ny,

 0 0 *,kS Mid - plan e - 4 5 -4.5 ",~.S 0 0

~Z mw

- 4 5

*t.5

 - 4 5 Mid-plane * `k5

Fig. 6.4 Symmetric (left) and non-symmetric (right) eight-ply laminates.

178 COMPOSITE MATERIALS FOR AIRCRAFT STRUCTURES

h n=t/2

 h k Ply k Tt h k-I ,.- y midplane h i Ply 2 1 Ply 1 h 0=-if2

Fig. 6.5 Ply coordinates in the thickness direction, plies numbered from the bottom surface.

and Ns, (Figure 6.6); the N are generally termed stress resultants and have the dimension "force per unit length." Elementary equilibrium considerations give

 n Nx = ~ O'x(k)(hk - hk-1), Ny = ~ O'y(k)(hk - hk-1), k = l k=l Ns = ~ Zxy(k)(hk - hk- 1) (6.11) k=l

Ny

l ~ Nxy

 't_ Nx X - 1

Fig. 6.6 Stress resultants.

 STRUCTURAL ANALYSIS 179

Substituting from equations (6.10) into (6.11), and remembering that the strains are the same in all plies, the following result is readily obtained:

 Nx = Axxex + Axyey + AxsYxy Ny = Axyex + Ayyey "t-Ays Yxy (6.12) Ns = Axsex -t'-Ayse,y + Ass'Yxy where: Aij = XZ, Qij( Ok)(hk -- hk-1) (6.13) k = l The quantities A o are the terms of the laminate "in-plane stiffness matrix."
 Given the single-ply moduli and the laminate lay-up details, they can be calculated routinely by using equations (6.4), (6.8), and (6.13). Equation (6.12) are generally taken as the starting point for any laminate structural analysis.

6 . 2 . 3 . 2 L a m i n a t e S t r e s s - - S t r a i n Law. As was just implied, it seems to be the current fashion in laminate mechanics to work in terms of the stress resultants, rather than the stresses. However, for some purposes, the latter are more convenient. From the stress resultants, the average stresses (averaged through the thickness of the laminate) are easily obtained; writing these stresses simply as o'x, try, and 7xy then:

 Nx Nx N, O ' x = - - , O'y = - - , "/'xy = - - ( 6 . 1 4 ) t t t

Hence, in terms of these average stresses, the stress-strain law for the laminate becomes:

 O-x = Axxex + Axyey "l- Axs ]txy Ory = Axy 8x -t- Ayy ~y --I-Ays 'Yxy (6.15) "rxy = A*xsex + Aysey + Ass'Yxy where: AU 1 (6.16) A~j = - - = - ~ Qij(Ok)(hk -- hk-1) t tk = 1

In some cases, equation (6.15) is more convenient than is equation (6.12).

6.2.3.30rthotropic Laminates. An orthotropic laminate, having the laminate axes as the axes of orthotropy, is one for which Axs = Ays = O ;

6.2.3.4 Modufi o f Orthotropic Laminates.

180 COMPOSITEMATERIALS FOR AIRCRAFT STRUCTURES

clearly, this implies that:

 n Qxs(Ok)(hk -- hk-l) = O, ~-~ Qys(Ok)(hk -- hk-1) = 0 (6.17) k = l k = l

Thus, the stress-strain law for an orthotropic laminate reduces to:

 O'x = Axxex + Axysy O'y = Axyex + Ayy~y (6.18) Txy = A,* Yxy The coupling between the direct stresses and the shear strains and between

the shear stresses and the direct strains, which is present for a general laminate, disappears for an orthotropic laminate. Most laminates currently in use are orthotropic.

It can be readily seen that the following laminates will be orthotropic:

(1)Those consisting only of plies for which 0 = 0 ° or 90°; here it follows from equation (6.8) that in either case Qxs(O) = Qys(0) = 0.

(2)Those constructed such that for each ply oriented at an angle 0, there is another ply oriented at an angle - 0; because, as already noted from the odd powers in equation (6.8),

Qxs( - O)= - Qxs(O) , Qys( - O)= - Qys(O )

There is then a cancellation of all paired terms in the summation of equation

(6.17).

(3)Those consisting only of 0 °, 90 °, and matched pairs of + 0 plies are also, of course, orthotropic.

An example of an orthotropic laminate would be one with the following ply pattern:

0 ° / + 3 0 ° / - 3 0 ° / - 3 0 ° / + 3 0 ° / 0 °

On the other hand, the following laminate (while still symmetric) would not be orthotropic:

0°1+30°190°190°1+30°/0°

Expressions for the moduli of orthotropic laminates can easily be obtained by solving equation (6.18) for simple loadings. For example, on setting try = "rxy= 0, Young's modulus in the x direction, Ex, and Poisson's ratio Vxy governing the contraction in the y direction

 STRUCTURAL ANALYSIS 181 for a stress in the x direction are then given by: O"x E y E x "= - - , P x y ~ - - - - ~ x ~'x Proceeding in this way, it is found that: *2 Ex = A*x , * A ~ Ey = Ayy -- - - Ayy A~ (6.19) Axy A~y G~y = As*~ Pxy "= Ayy-'T Yyx ~ ~xx

As illustrative example s o f the above theory, consider a famil y o f 24 - ply laminates, symmetrica l and orthotropic, and all mad e of the same materia l but with varyin g numbers o f 0 ° and _ 45 ° plies. (Fo r the present purposes, the precise ordering o f the plies is immateria l as long as the s y m m e t r y requiremen t is maintained; however, to ensure orthotropy, there mus t be the same numbe r o f

 + 45 ° as - 4 5 ° plies.) The single - pl y modulu s data (representative o f a c a r b o n / epoxy) are: El = 137 . 44GP a E2 = 1 1 . 7 1 G P a Gt2 = 5 . 5 1 G P a ]212 = 0.2500 V 2 1 = 0.0213 (6.20)

The lay - up s considere d are shown in Table 6.1. The steps in the calculation are as follows:

 (1) Calculat e the Qij(O) fro m equation (6.4). (2) Fo r eac h o f the pl y orientations involve d here 0 = 0 °, + 4 5 °, and - 4 5 °, calculate the Qij(O) fro m equation (6.8). [Of course, here the Qo(O) have alread y bee n obtained in step 1.] Table 6.1 Moduli for Family of 24-ply 0°/+_ 45° Laminates Constructed Using Unidirectional Tape Lay-up No. 0° No. + 45 ° No. - 4 5 ° Ex, Ey, G~, l~xy ])yx Plies Plies Plies GPa GPa GPa 24 0 0 137.4 11.7 5.51 0.250 0.021 16 4 4 99.4 21.1 15.7 0.578 0.123 12 6 6 79.5 24.5 20.8 0.647 0.199 8 8 8 59.6 26.4 25.8 0.693 0.307 0 12 12 19.3 19.3 36 0.752 0.752

182COMPOSITEMATERIALSFOR AIRCRAFTSTRUCTURES

(3)Calculate the A,~ from equation (6.16); in the present case, equation (6.16) becomes:

Aij = [nlQo(0) + neQij(+45) + n3Q(i(-45)]124

where nl is the number o f 0 ° plies, n2 o f + 4 5 ° plies and n3 o f - 4 5 ° plies.

(4) Calculate the moduli from equation (6.19).

The results o f the calculations are shown in Table 6.1.

The results in Table 6.1 have been presented primarily to exemplify the preceding theory; however, they also demonstrate some features that are important in design. The stiffness of a composite is overwhelmingly resident in the extensional stiffness o f its fibers; hence, at least for simple loadings, if maximum stiffness is required, a laminate is constructed so that the fibers are aligned in the principal stress directions. Thus, for a member under uniaxial tension, a laminate comprising basically all 0 ° pries would be chosen; in other words, all fibers would be aligned parallel to the tension direction. As can be seen from Table 6.1, Ex decreases as the number o f 0 ° plies decreases. On the other hand, consider a rectangular panel under shear, the sides o f the panel being parallel to the laminate axes (Fig. 6.7a). The principal stresses here are an equal tension and compression, oriented at + 4 5 ° and - 4 5 ° to the x-axis. Thus, maximum shear stiffness can be expected to be obtained using a laminate comprising equal numbers o f + 4 5 ° and

 - 4 5 ° plies; this is reflected in the high shear modulus G,:y for the all _+ 45 ° laminate o f Table 6.1. ÷~5" Fibre Fibre 'L_ \ \ \\//../ 5 " ~ X iii / ' \ -~,s'/-'-7 \\4 a) (i) Shearpanel (ii) Principal stresses (iii) Fibredirections

L_

x

b)

 " )~",. / \ ./",. IX./',,. /"y'l"""'*" ..__D - ' ~ -- ' - ~' - ' - 2~C'"~'~- - ~ 7 ,,,_l = :x = 68.9 MPa .,> I(-×.~X ,X.~X~,~.,~5<.NX-)I__,. ...~... v '~./ \ / , J ~ / \ / V X J ~

Fig. 6.7 Ply orientations for example problems: a) fiber orientations for a shear panel: b) 0° _ 45 ° laminate under uniaxial tension.

 STRUCTURAL ANALYSIS 183

It should also be observed that, although for an isotropic material, Poisson's ratio cannot exceed 0.5, this is not the case for an anisotropic material.

6.2.3.5 Quasi-lsotropic Laminates. It is possible to construct laminates that are isotropic with regard to their in-plane elastic properties---in other words, they have the same Young's modulus E and same Poisson's ratio v in

 all in-plane directions and for which the shear modulus is given by G = E / 2 ( l + v ) . One way of achieving this is to adopt a lay-up having an equal

number of plies oriented parallel to the sides of an equilateral triangle. For example, a quasi-isotropic 24-ply laminate could be made with 8 plies oriented at each of 0 °, + 60 °, and - 60 °. Using the same materials data (and theory) as were used in deriving Table 6.1, it will be found that such a laminate has the following moduli:

E = 5 4 . 2 G p a , G = 2 0 . 8 G p a , v = 0 . 3 0 5

Another way of achieving a quasi-isotropic laminate is to use equal numbers of plies oriented at 0 °, -t-45 °, - 4 5 °, and 90 °. A quasi-isotropic 24-ply laminate (with, incidentally, the same values for the elastic constants as were just cited) could be made with 6 plies at each of 0 °, + 4 5 °, - 4 5 °, and 90 °. (For comparison, recall that Young's modulus and the shear modulus for a typical aluminum alloy are of the order of 72 and 27 GPa, respectively, and that the specific gravity of carbon/epoxy is about 60% that of aluminum.)

The term quasi-isotropic is used because, of course, such laminates have different properties in the out-of-plane direction. However, it is not usual practice to work with quasi-isotropic laminates; efficient design with composites generally requires that advantage be taken of their inherent anisotropy.

6.2.3.6 Stress Analysis of Orthotropic Laminates. The determination of the stresses, strains, and deformations experienced by symmetric laminates under plane stress loadings is carried out by procedures that are analogous to those used for isotropic materials. The laminate is treated as a homogeneous membrane having stiffness properties determined as described above. It should be noted, though, that while the strains and deformations so determined are the actual strains and deformations (within the limit of the assumptions), the stresses are only the average values over the laminate thickness.

If an analytical procedure is used, then generally a stress function F is

 introduced, this being related to the (average) stresses by 02F OZF - 02F (Eq. 6.21) O"x -~- OX2 , O'y = 0)22 , T r Y - OxOy

184 COMPOSITE MATERIALS FOR AIRCRAFT STRUCTURES

It can be shown that F satisfies the following partial differential equation:

 ( 1 ) 04F ( 1 2Vxy'~ 04F ( 1 ) O4F ~y ffx~-+ ~-y ~ - ) 3 x - - 5 - ~ + ~ - ~ - - = 0 (6.22)

Solutions of equation (6.22) for several problems of interest can be found in Ref. 10.

Most structural analyses are now performed using finite element methods described in Chapter 16, and many general-purpose finite-element programs contain orthotropic membrane elements in their library. Once the laminate moduli are determined, they are used as input data for calculating the element stiffness matrix; the rest of the analysis proceeds as in the isotropic case.

As has already been emphasized, the stresses obtained from the above procedures are only the average stresses. To determine the actual stresses in the individual plies, it is necessary only to substitute the calculated values of the strains in equation (6.10). An elementary example may clarify this. Consider a rectangular strip under uniaxial tension (Fig. 6.7b) made of the 24-ply laminate considered earlier that had 12 plies at 0°, 6 plies at + 4 5 °, and 6 plies at - 4 5 °. Suppose the applied stress is ~rx = 68.9 MPa. The average stress here is uniform in the xy plane and given by:

o-x = 68.9 MPa, O'y = Ts = 0

Using the values of Ex and Vxy given in Table 6.1, it follows that the associated strains are:

ex = 0.8667 x 10-3, 8y = - 0 . 5607 x 10-3, % = 0

The stresses in the individual plies can now be obtained by substituting these values into equation (6.10), with the appropriate values of the Qij(O). The results of doing this are shown in Table 6.2.

Thus, the actual stress distribution is very different from the average one. In particular, note that transverse direct stresses and shear stresses are developed, even though no such stresses are applied; naturally, these stresses are self-equilibrating over the thickness. It follows that there is some "boundary layer" around the edges of the strip where there is a rapid transition from the actual stress boundary values (namely, zero on the longitudinal edges) to the calculated values shown in the table. This boundary layer would be expected to extend in from the edges a distance of the order of the laminate thickness (from the Saint-Venant principle). In the boundary

Table 6.2 Stresses in Individual Plies of a 24-Ply Laminate (12 at 0% 6 at

 + 45 a n d 6 a t - 45 °) under Uniaxial Stress of 68.9 M P a 0 ° Ox(O) M P a o~v (0) M p a "rxy(O) M P a 0 118.1 - 4 . 1 0 + 4 5 19.8 4.1 9 . 7 - 4 5 19.8 4.1 - 9 . 7
 STRUCTURAL ANALYSIS 185

layer, the simple laminate theory presented above is not applicable and a threedimensional analysis is required. The matter is of more than acad6mic interest since faults, such as delaminations, are prone to originate at the free edges of laminates because of the above effect. Edge effects will be considered further in Section 6.3.2.

Finally, when discussing allowable design values for composite structures, it is common to cite values of strain, rather than stress. Clearly, strain is the more meaningful quantity for a laminate.

6.2.3.7 Laminate Codes. Although the precise ordering of the plies of a laminate has not been of concern in the considerations of this section, generally there will be other factors that will determine such an ordering. In any case, when a laminate is being called up for manufacture, the associated engineering drawing should list the orientation of each ply. When referring to laminates in a text, some sort of abbreviated notation is necessary to specify the pattern. It is easiest to describe the code normally used with some examples.

Example 6.1

Consider an eight-ply uni-directional tape laminate with the following (symmetric) lay-up starting from the bottom (z = t/2) surface:

0 ° / 0 ° / + 4 5 ° / - 4 5 ° / - 4 5 ° / + 4 5 ° / 0 ° / 0 °

This is written in code form as:

[02/ _+ 45]s

Note that:

(1)Only half the plies in a symmetric laminate are listed, the symmetry being implied by the s outside the brackets.

(2)The degree signs are omitted from the angles.

(3)In a -4- and - combination, the upper sign is read first.

Example 6.2

Consider a four-ply fabric laminate with the following (symmetric) lay-up: (0°,90°)/( ___45°)/( _ 45 °)/(0°, 90°).

This is written in code form as

[ ( 0 , 9 0 ) / ( + 4 5 ) / ( 0 , 9 0 ) ] or [(0,90)/(_+15)].

Example 6.3

Consider a fifty-ply tape laminate containing repetitions of the ply sequence: 0 ° / 0 ° / + 4 5 ° / - 45o/90 o

186 COMPOSITE MATERIALS FOR AIRCRAFT STRUCTURES

The order in the sequence being reversed at the midplane to preserve the symmetry. This would be written in code form as:

[(02/ _ 45/90)5]s

Sometimes, in general discussions, a laminate is described by the percentages of its plies at various angles. Thus, the laminate of example (6.1) would be described as having "50% 0, 50% +_45." Similarly, the laminate of example (6.2) would be described as having "40% 0, 40% _ 45, 20% 90."

6.2.4General Laminates Subjected to Plane Stress and Bending Loads

In this section the previous restriction to laminates that are symmetric about the mid-thickness plane will be dropped. It now becomes necessary to consider the plane stress and bending problems in conjunction, as in-plane loads can induce bending deformations and vice versa. Only the outline of the theory will be given below; for further details, including numerical examples, see Refs. 1-5.

6.2.4.1 General Theory. In contrast to the situation for symmetric laminates, the position of each ply in the laminate is now important. Thus, consider an n-ply laminate with z the coordinate in the thickness direction, measured from the mid-thickness plane. The kth ply lies between hk_ 1 and hk (Fig. 6.5). As before, the total thickness of the laminate will be denoted by t.

It is assumed that when a laminate is subjected to in-plane and/or bending loads, the strain varies linearly through the thickness and can therefore be written in the form:

 ~x = o ~Y = o jr KyZ ]/xy = ~y + KsZ (6.23) ~x "~- KxZ ~y where the superscript o quantities are the mid-plane strains and the Kt are the

midplane curvatures (as in the bending of isotropic plates). Both these sets of quantities are independent of z.

Substituting from equation (6.23) into equation (6.7), it follows that the stresses in the kth ply will now be given by:

Orx(k) ~ axx( Ok)(~° Jr ZKx) "~- axy( Ok)(~; Jr ZKy) Jr axs( Ok)(~xy Jr ZKs) try(k)=axy(Ok)(8 ° -}-ZKx)q-Qyy(Ok)(~y Jr-ZKy)+Qys(Ok)(~xy -~-ZKs) (6.24)

~'xy(k) = axs( Ok)(8° Jr ZKx) -~-ays( Ok)(~y Jr ZKy) -~ ass( Ok)(~xy + ZKs)

 STRUCTURALANALYSIS 187

Now introduce the stress resultants (in the form of forces per unit length and moments per unit length) defined by:

(6.25)

 where all of the integrals are over the thickness of the laminate (i.e., from z = - t/2 to z = t/2); see Figure 6.8. Because each of the integrals in equation (6.25) can be written in forms such as: n r h k n c h k (6.26)

it follows that substituting from equation (6.24) into equation (6.26), and performing some elementary integrations, leads to the result:

 Axx Axy Axs Bxx Bxy Bxs] Axy Ayy Ays Bxy Byy Bys A~ Ays Ass Bx~ Bys Bss LBxx Bxy Bxs Dxx Dxy Dxs Bxy nyy Bys Dxy Dry Oys Bxs Bys Bss Dxs Dys Dss

o 13x

 I] o Uy = N~ (6.27) m~ Ky K s m~

Ny

zt ,

 / ~ Nxy

Nx

X

.I_

t

T

My

Fig. 6.8 Stress an d m o m e n t resultants for a laminate.

188 COMPOSITE MATERIALS FOR AIRCRAFT STRUCTURES

The elements in the above combined "extensional-bending stiffness matrix" are given by:

 n Aij = E Qij(Ok)(hk -- hk-1) (6.28) k = l Bij = ~ aij(Ok)(h 2 - h2_1)/2 (6.29) k = l n Dij = ~ Qij(Ok)(h3 - h3_t)/3 i, j = x, y, s (6.30)

k = l

[The above definition for Aij, is, of course, equivalent to that of equation (6.13).] Equation (6.27) can be used to develop a theory for the stress analysis of general laminates, but this is quite formidable mathematically. It involves the solution of two simultaneous fourth order partial differential equations.

6.2.4.2 Uncouplingof the StiffnessMatrix. It can be seen from equation

(6.27) that the plane stress and bending problems are coupled unless all the Bij, are zero. It follows from equation (6.29) that the Bij are indeed zero for a symmetric lay-up. [For a symmetric pair of plies, if that ply below the mid-plane has coordinates hk- 1 ---~ - - a and hk = - b, then its mate above the mid-plane will have h k _ 1 = b and hk = a. Because each ply has the same Qi.i, there is a cancellation in the summation of equation (6.29).]

It is possible to achieve an approximate uncoupling of equation (6.27) for a multi-ply unsymmetric laminate by making it in the form of a large number of repetitions of a given ply grouping. It can be seen intuitively that such a laminate will be symmetric in the group of plies if not in the individual plies; as long as the number of plies in the group is small compared with the total number of plies in the laminate, the Bij, will turn out to be small quantities. For example, a 48-ply laminate containing 24 groups of 45 ° plies laid up in the sequence + / - / + / - etc. (without there being symmetry about the mid-plane) would be expected to behave much as a symmetrical laminate of the same plies.

6.2.4.3 Bending of Symmetric Laminates. The moment-curvature relation governing the bending of symmetric laminates out of their plane, as

 extracted from equation (6.27), is: oslEKyj [ox Oyy = M y . Oxy Oys ( 6 . 3 1 ) Dxs Dys Dss_l Ks Ms

Analogously to the definition of orthotropy in plane stress, a laminate is said to be orthotropic in bending if Dxs = Dys = 0. However, it is important to note that a laminate that is orthotropic in plane stress is not necessarily orthotropic in

 STRUCTU RAL ANALYSIS 189 bending. For example, consider the four-ply laminate [___45]~. Here the coordinates for the +45 ° plies may be written as ( - t/2, - t/4) and (t/4, t/2), whereas those of the - 45 ° plies are ( - t/4, 0) and (0, t/4); t, of course, is the

laminate thickness. It is easy to establish that, while Ax~and Ay s are zero, Dx~ and Dys are not. On the other hand, a laminate, containing only 0° and 90° plies will be orthotropic in both plane stress and bending. These laminates are called specially orthotropic. (It is also worth noting that for multi-ply laminates made of groups of plies, if the group is orthotropic in plane stress, then the laminate will at least be approximately orthotropic in both plane stress and bending.)

As an example, consider the bending of the simply-supported beam shown in Figure 6.9a under a uniform distributed load. The laminate consists of a lay-up [04 904]s. Using the single-ply modulus data given in equation (6.20) and a ply

 thickness of 0.125 mm, equation (6.31) becomes: E81584,9621.962 18.382 0.0oolExIKy = My Nm/m (6.32) 0.0 0.0 3.673 K~ Ms If the moment per unit width at the center of the beam is Mx = 100 N/m, My = Ms = 0, solving for the curvature gives Kx = 1.229, Ky = --0.131, and

Ks ----0.0, indicating the anti-elastic curvature effect typical of plates. Solving for strains in the laminate involves substituting in equations (6.23) and (6.24) with zero for the mid-plane strains. The stress and strain through the thickness are given in Figure 6.9b.

 q I I a) z z l m m ~ 1 m m ~ 169 MPa I / 7 MPa - ~ 1229 ~E I~x / ~ (Yx - l m m -1 m m

Fig. 6.9 Configuration and results for simply-supported beam.

190 COMPOSITEMATERIALS FOR AIRCRAFT STRUCTURES

To estimate the deflection at the center of the beam, the matrix of coefficients in equation (6.32) is inverted to give:

 ICy : dxy dyy dys My Ks dxs dys dss Ms o.o l[ xl [o.o19 _o.oo131 = -0.00131 0.05454 0.0 My rad/m 0.0 0.0 0.27223 Ms

In simple beam theory, a total moment M applied to a beam gives the curvature that satisfies the equation:

 d2w M Kx-- dx 2 E1

Imposing a moment per unit width on the laminate Mx = M/b , My = Ms = 0 on the laminate of width b, then dx~/b = 1/(E/)effective. This effective bending stiffness can be substituted in the simple beam relation 6 = 5qL 4/384EI, where q is the load per unit length applied to the beam, to obtain a first order approximation of the deflection of the laminate.4 For short beams, the simple bending theory is inaccurate, and shear deformation needs to be included.

Composite beams are often stiffened using a lightweight core of Nomex honeycomb or expanded foam. 11 The laminate can be analyzed by including a layer in the center of the laminate with negligible in-plane properties. Use of the laminate theory implies that the core material has sufficient transverse shear and through-thickness compression stiffness to ensure that the top and bottom skins and the core material are constrained to behave as an integral laminate. Repeating the calculation with a 10-mm core added at the center of the previous laminate

 gives the DO indicated in the following equation: ?1 4896.046 00 l[ xl 178.552 4200.829 0.0 % = My Nm/m 0.0 0.0 334.273 Ks Ms

which represents an increase of bending stiffness approaching two orders of magnitude.

For an orthotropic plate in bending, the deflection w satisfies the following equation:

 D Ow 2(Dxy+2Dss) °4w D 0 w-- xx'~'q' - ~X~-~-{'- y y " - ~ -- q

where q is the applied pressure. Solutions of this equation can be found in Ref. 3. In this reference, the related problem of the buckling of laminated plates is also discussed.

Тут вы можете оставить комментарий к выбранному абзацу или сообщить об ошибке.

Оставленные комментарии видны всем.

Соседние файлы в предмете [НЕСОРТИРОВАННОЕ]